Skindeep - 39 - Leather Manufacturers and Bookbinding How to Read Bookbinding Leather...
Embed Size (px)
Transcript of Skindeep - 39 - Leather Manufacturers and Bookbinding How to Read Bookbinding Leather...
Skin Deep The Biannual Newsletter from J. Hewit & Sons Ltd. No.39 Spring 2015
How to Read Bookbinding Leather Page 2
A practical guide by book conservator, Karen Vidler
J Hewit & Sons: A Company History Page 14
Part 1 - The first 50 years by Roger Barlee
Was there a shortage of Goats in Roman Britain Page 32
.....or where have all the Goats gone?
Product & Company News Page 9
Study Opportunities Page 19
Customers Recent Bindings Page 28
Dates for your Diary Page 30
How to Read Bookbinding Leather
by Karen Vidler
When choosing leather for a new bookbinding or book repair an understanding of this material can assist in deciding on the best leather for the job. This includes recognising the animal species, how the leather was tanned and dyed and whether the leather was finished with a pigmented and embossed surface finish. These are just some of the processes that influence the final look, workability and durability of leather for bookbinding. Bookbinding leather making requires a series of physical and chemical processes than can be broken down into three fundamental stages: 1. Removal of unwanted material such as hair, flesh,
fat, interfibrillar (within the fibres) materials leaving a network of high protein collagen fibres, softened and interspaced with water 2. Tanning or treating the skin with a tanning agent to displace some of the water and combine with and coat the collagen fibres. Tanning increases the skins resistance to heat, hydrolysis (decay involving water) and microbial attack and 3. Finishing: where the final required thickness and appearance is achieved for the end use of the leather such as bookbinding. Finished Leather at J Hewit & Sons
Structure of Animal Skin A skin of leather can be divided into different areas to help understand why the leather responds the way it does during the book covering process. Mammalian skins used for bookbinding leather have specific areas that indicate the arrangement of the leather fibres during the life of the animal and the final leather properties. The more elastic areas are where the animal skin stretches such as during movement or increasing weight. This includes the legs, neck and belly regions. The less elastic areas are dimensionally more stable such as the shoulders and butt. In the illustration below these areas are labelled across a mammalian skin. The red areas of the Daniels diagram indicate the optimum selection area for bookbinding and book repair purposes based on measured tensile strength and stretch. Labelled diagram of mammalian leather
R. Daniels contour map of leather performance
based on E. Swasyland data
The collagen fibres are arranged into fibre bundles in a woven network running through the thickness of the skin. As can be seen in the well-known cross section diagram by Sharphouse, fibres are arranged into three distinct layers common to all mammals used for bookbinding leather. 1. The upper layer is the all-important grain that the tanner seeks to preserve 2. The central corium layer which is the strongest section of the skin structure 3. The flesh layer of which most is removed during the early stages prior to tanning as this is not required for the final leather. The fibre bundles become more ordered with an increasingly shallow angle of weave as they move from the flesh through the corium to the grain layer of the skin. The hair shafts pass through the skin at varying depths depending on the animal species.
Leather cross section J.H. Sharphouse Leather Technicians Handbook, 1971
SEM image of unravelling calf leather fibres
The most commonly used animal species for bookbinding leather include calf, goat, sheep skin and kangaroo and can be ranked for durability. Species recognition can be done following some basic characterisations of each skin and examination with a hand magnifier and lots of practice.
Calf skin is characterised by a hair follicle pattern within the skin surface that is evenly sized and spaced along the grain layer with no distinct pathways. The skin has relatively straight and shallow hair shafts that do not interrupt the junction between the grain and corium with uniform fibre bundles through the corium into the grain to impart strength through the leather. But the fibres are arranged at a steep angle so paring will reduce the strength of the final leather at the grain and corium junction. The grain pattern of goat skin consists of clusters of large guard hairs and small fine hair follicles running in wide pathways across the surface of the skin. The skin structure has an even distribution of fibre bundles throughout the corium and grain and a shallow angle of entry of the guard and fine hair follicles which are evenly spaced throughout the skin. Goat skin leather is considered a durable animal skin for bookbinding purposes because of this strong internal structure. The grain pattern of hair and wool sheep can be difficult to identify as like goat skin they contain clusters of large guard hairs and small fine hair follicles. Sheep skin is the least durable animal skin for bookbinding leather purposes due to the location of sebaceous (fat) glands that lubricate along the hair shaft being located at the grain and corium junction which leave a looseness to the final leather after tanning. Also sheep skin has been, in recent history, tanned and surface finished with materials and processes that have ensured the leather is less durable over time. Kangaroo skin has a distinct grain pattern of even sized, fairly straight and narrow hairs arranged in clusters of three or four fine hairs. Clusters run in long pathways across the skin. Internally the fibre bundles are evenly distributed at a low angle of weave with a highly uniform orientation of fibre running almost parallel with the skin causing a high tensile strength between grain and corium. Kangaroo has a thin grain and thick corium layer so paring will not greatly reduce the final strength of the leather. For these reasons Kangaroo is considered to make the most durable leather for bookbinding if tanned and finished correctly. Tanning Materials The other main raw material for bookbinding leather making is the vegetable tanning material. A vegetable tannin can be defined as an astringent mixture (quick to bind) of plant polyphenols and non-tannins that chemically bond to the collagen fibres and sourced from barks, leaves, roots and seed pods. The non-tans include sugars, starches, salts and acids that enter the leather, but do not directly react with the collagen fibres. They are thought to be important as they influence the progress of both tanning and the final qualities of the leather such as degree of water resistance, firmness and resistance to atmospheric pollution.
Oak Bark sourced from Mimosa sourced from Sumac source from Great Britain and Europe South Africa and Australia Africa and Mediterranean
Traditionally bookbinding leather was tanned with oak bark. With the increased shortage of this raw material in the 18th century new tannins were investigated at a time when the British Empire was exploring the New World. At the same time as the discovery of alternative tanning materials, the discipline of leather chemistry was developing and this led to an understanding of the difference between these agents. Vegetable tannins can be divided into two groups commonly referred to as the condensed and the hydrolysable groups. The condensed tannins impart a reddish-brown colour to the tanned skin. They are very astringent so penetrate and fix to the collagen fibres quickly so are more popular tanning agents. The red colour is due to the high amount of the phlobaphene compound present in the tannin that reacts quickly to form red products in leather. Condensed tannins are more effective sinks for sulphur dioxide adsorption (on the surface) from acid gas pollution so acid decay is more aggressive. These tannins include Mimosa, Quebracho, Mangrove and Hemlock. The hydrolysable tannins have been described in the research as the good tans for making more durable bookbinding leather. Usually a yellow-olive or yellow-brown colour is imparted in the tanned skin. This is a less astringent group of tannins so penetration and fixation is generally slower. The tanned leather is thought to contain more carbohydrates or salts (non-tans) which assist in making the skin more resistant to ageing from heat, light and gaseous pollutants. Examples include Sumac, Myrabolans, Chestnut, Valonia and Tara. Oak bark is considered a mix-tan. Tanning Process
Pit tanning was the common vessel for vegetable tanning groups of skins together prior to the 19th century. These pits were based on the counter-current system whereby skins are put into an old, almost exhausted tanning liquor, then progress through a series of pits of increased strength liquor to fix more tans at a controlled rate. There is very little movement or mechanical action of the skins apart from gentle agitation and the cycle of lifting the skins to inspect and move from one pit to the next. Claytons Pit tanning
This system was gradually replaced by the drum tanning method in the mid-18th century or possibly earlier. Modern tanning drums have shelves or spokes that catch the skin during the tanning process which hold it in the air and allow it to drop with some force as the drum turns. This mechanical action squeezes and compresses the skin increasing the rate of penetration of